Tea Dust Recipes on Glazy
The following glazes and more can be found on my new website, Glazy:
The Complete Guide to High Fire Glazes Tea Dust Recipes
Some tea dust glazes from The Complete Guide to High Fire Glazes. I fired these glazes according to my usual firing schedule, probably too hot and not ideal for the development of crystals necessary for good tea dust glazes. I crash cool to 1000C and then completely shut up the kiln.
Currie 10 Tea Dust
Currie 11 Tea Dust
Coleman Tea Dust
Tea Dust Black
Tessha Tea Dust
Chinese Traditional Tea Dust Glaze
Although the glazes above call all be considered tea dust, in China teadust glaze usually refers to Qing dynasty wares like the ones below. Although tea dust can result in a range of colors and with varying crystal sizes, usually the crystals are very evenly dispersed. (The example below is a Qianlong vase sold through Sotheby’s.)
Qianlong Teadust Vase
Various Teadust Colors
Chinese Traditional Tea Dust Glaze Recipes
The recipe above comes from 颜色釉 (Colored Glazes), published in 1978 by the Jingdezhen Ceramics Company. The components of the recipe can be difficult to find today, even in Jingdezhen. Those materials that are still produced probably have different compositions than in 1978. For instance, I’ve noticed differences in Glaze Stone (釉果) and Zijin Stone (紫金石) from year to year. What this recipe has in common with the Western tea dust glazes above is the addition of magnesium oxide in the form of talc, which helps form the tea dust crystals.
The glaze preparation is quite interesting. The ingredients (excluding the white clay (白土)) is ball milled for 30 hours, then white clay is added and the full glaze is milled for another four hours. After adding water, the glaze is sprayed approximately 1mm thick. Firing is to 1250°C in a weak reduction atmosphere.
Tea Dust Triaxial - First Attempt
In part because I’ve had a difficult time finding a reliable chemical analysis for the glaze stone I use, but mostly because I often don’t have much clue what I’m doing, I often use triaxial blends to find interesting glazes. I’m also interested in making glazes for my normal firing schedule, rather than changing my firing for a single type of glaze (like the recipe above that fires to 1240°C).
Because triaxials are limited to three variables, the following tests make some assumptions about tea dust glazes. The top axis of the triaxial will be glaze stone (the “unknown” ingredient), the left axis whiting (the flux), and the right axis silica. I’m certain I need magnesium in the form of talc, dolomite, or magnesium carbonate- I choose 8% talc. I also need some iron, based on past experience and other glaze recipes I choose red iron oxide at 8%.
From the resulting triaxial it seems that crystal growth improves as silica is increased while glaze stone and whiting are decreased.
Tea Dust Triaxial - Second Attempt
For each row of the first triaxial, I like what’s happening in the third column. For the next test, I extend this third column down a few rows to see what happens.
It’s nice to see my educated guesses are working out. Beginning from the fourth row of this second test, it seems like I’m coming close to a glaze that I like.
You’ll notice that the glazes look completely different on the two types of test tiles (porcelain on the left and stoneware on the right).
Just to check that my initial amounts for Iron and Talc are in the right ballpark, I choose the fourth row of this test and make some adjustments. It seems that Red Iron Oxide at 8% additional and Talc at 10% are ideal.
After a few more tests further adjusting the silica, iron, and talc I ended up with the glaze at the left. While it’s not an ideal tea dust glaze by Qianlong standards, what’s important is that I like it and I can fire it using my usual temperature and schedule.
August 2015 Update
Just to see what would happen if I continued adding silica to the recipe, I extended the bottom-right corner of the original triaxials. As you can see below, incrementally replacing glaze stone with silica leads to an increasingly uniform crystal distribution more closely approximating Chinese teadust glazes. (A feldspar/whiting/silica triaxial for some of the High-Fire Glazes recipes above may have similar results.) Note that in the following tests I increased Red Iron Oxide to 9% (additional).